Enhanced Catalytic Activity of a New Nanobiocatalytic System Formed by the Adsorption of Cytochrome c on Pluronic Triblock Copolymer Stabilized MoS2 Nanosheets

The formation of nanobiohybrids through the immobilization of enzymes on functional nanomaterials has opened up exciting research opportunities at the nanobiointerfaces. These systems hold great promise for a wide range of applications in biosensing, biocatalytic, and biomedical fields. Here, we report the formation of a hybrid nanobiocatalytic system through the adsorption of cytochrome c (Cyt c) on pluronic triblock copolymer, P123 (PEO-b-PPO-b-PEO), stabilized MoS2 nanosheets. The use of pluronic polymer has helped not only to greatly stabilize the exfoliated MoS2 nanosheets but also to allow easy adsorption of Cyt c on the nanosheets without major structural changes due to its excellent biocompatibility and soft protein-binding property. By comparing the catalytic activity of the Cyt c–MoS2 nanobiohybrid with that of the free Cyt c and as-prepared MoS2 nanosheets, we have demonstrated the active role of the nanobiointeractions in enhancing the catalytic activity of the hybrid. Slight structural perturbation at the active site of the Cyt c upon adsorption on MoS2 has primarily facilitated the peroxidase activity of the Cyt c. As the MoS2 nanosheets and the native Cyt c individually exhibit weaker intrinsic peroxidase activities, their mutual modulation at the nanobiointerface has made the Cyt c–MoS2 a novel nanobiocatalyst with superior activity.


INTRODUCTION
The discovery of a two-dimensional (2D) layered graphene nanomaterial opened up an area of intensive research due to its exceptional mechanical strength, high thermal and electrical conductivity, and optical properties. 1−4 Since then, graphenelike 2D nanosheet materials such as transition metal dichalcogenides (TMDCs), graphitic carbon nitride, MXenes, hexagonal boron nitride (h-BN), and transition metal oxides (TMOs) have become the center of attention. 5 2D layered materials (single or few layers) are more fascinating than their bulk form because of the high density of active surface sites available over a large area. 6 A broad range of electronic properties like metallic/semimetallic (e.g., graphene, VS 2 , TaS 2 ) to semiconducting (e.g., MoS 2 , WS 2 ) or insulating (e.g., h-BN) properties are exhibited by them. 4,5 Similarly, they have a broad range of optical properties like fluorescence quenching or emission behavior. 7,8 2D molybdenum disulfide (MoS 2 ) is one of the pioneers of TMDC materials with an excellent layer-dependent band structure. 9,10 A direct band gap of ∼1.8 eV possessed by the monolayer MoS 2 nanosheet makes it a good semiconducting material, resolving the gapless problems of graphene. 11 A single MoS 2 nanosheet is composed of a layer of Mo atoms sandwiched between two layers of S atoms. Strong covalent bonding between Mo and S atoms strengthens the trilayer MoS 2 nanosheet, and a weak Van der Waal force stacks them up. The MoS 2 nanosheet can have two distinct crystalline phases at room temperature, one with trigonal prismatic coordination, which is found to be semiconducting (2H), and the other one with octahedral coordination (1T), which is metallic. MoS 2 nanosheets have gained burgeoning interest in biosensor, biocatalytic and biomedical applications specifically due to their unique optoelectronic properties, high capacity of biomolecule loadings and good biocompatibility. 12−19 Moreover, their tailoring behavior to selectively respond to specific analytes with high sensitivity through different surface functionalizations has led to their extensive usage in biosensing and biocatalytic applications. 20,21 Although natural enzymes can perform catalytic activity with high efficiency and selectivity, they often require strict reaction conditions like specific temperature, pH, and ionic strength. The instability of natural enzymes under drastic conditions limits their industrial applications. 22 To overcome these limitations, researchers are now focusing on the development of new low-cost, stable, and active nanobiocatalytic systems by interfacing natural proteins/ enzymes on a wide variety of functional nanomaterials (or nanozymes). 23 In this work, we have demonstrated superior catalytic performance of a new Cyt c−MoS 2 nanobiocatalytic system developed by interfacing Cyt c on triblock copolymer P123 stabilized MoS 2 nanosheets (Scheme 1).
The MoS 2 nanosheets used in this work were synthesized via the ultrasonication-assisted liquid-phase exfoliation method. 10 This method provides a simple but effective route for obtaining sufficient quantities of thin-layered MoS 2 nanosheets with high structural quality. This method has previously been extensively employed using various types of surfactants and polymers as dispersants to yield MoS 2 nanosheets/nanoparticles of varying sizes and thicknesses. 10,24,25 Here we have used 1% (w/v) aqueous solution of a pluronic triblock copolymer, P123, as an effective dispersant for the exfoliation of bulk MoS 2 . P123 is a nonionic amphiphilic triblock copolymer composed of hydrophobic poly(propylene oxide) (PPO) and hydrophilic poly-(ethylene oxide) (PEO) blocks. The choice of P123 was made based on the biocompatible nature of the polymer and its preventive role toward aggregation or the major structural change of proteins after adsorption on nanomaterials. 26 The large molecular weight of the polymer and its long hydrophobic and hydrophilic chains also provides effective stabilization to the exfoliated MoS 2 nanosheets by capping on their surface. The hydrophobic PPO units can be adsorbed on the MoS 2 nanosheets, while the hydrophilic PEO polymer chains remain extended into the bulk solution (Scheme 1). These hydrophilic chains provide effective steric hindrance to prevent flocculation or aggregation of the nanosheets. 27−30 Apart from providing a biocompatible environment, the polymer chains on MoS 2 nanosheets also play an important role in anchoring more Cyt c on the nanosheets for enhanced catalytic activity of the hybrid.
Cytochrome c (Cyt c) is a globular heme protein which functions as an electron carrier for oxidative phosphorylation (or mitochondrial respiration) in the inner mitochondrial membrane of healthy cells. 31,32 The Fe center of Cyt c is six coordinated in its native state with methionine (Met 80) as a distal ligand. 33 The protein chain of Cyt c consists of 104 amino acids with an isoelectric point of ∼10 (due to the presence of a large number of basic amino acids like lysine). Hence, Cyt c bears positive surface charge at physiological pH. 32 Although Cyt c primarily functions as an electron carrier in its native state, under pro-apoptotic (programmed cell death) conditions it gains peroxidase activity in the presence of H 2 O 2 . 31,34,35 Certain conformational change of Cyt c induced by its interactions with membrane-bound cardiolipin is believed to be responsible for gaining in vivo peroxidase activity. 36 However, the exact nature of the conformation and the mechanism by which it gains peroxidase activity still remain elusive. Classical peroxidases have a five-coordinate heme structure, and the sixth coordination of the iron center is either vacant or occupied by a loosely bound water molecule. 37 This structural feature facilitates the interaction of H 2 O 2 with the iron center. Peroxidases generally follow a mechanism in which H 2 O 2 reacts with the Fe(III) resting state of heme to produce an oxyferryl compound (Fe(IV)O heme) known as Compound I along with an adjacent radical. The resting state of enzymes is regenerated with the abstraction of hydrogen from organic substrates, and the newly formed radical then yields stable oxidation products upon reactions with O 2 . 34 The native Cyt c becomes a potent peroxidase only after some conformational changes (or after the formation of a partially unfolded structure) with the weakening or rupturing of the Met80 S−Fe bond. 32,34 The improved peroxidase-like catalytic activity of Cyt c has been extensively investigated using a wide variety of supporting materials such as polymers, 38 graphene oxide nanosheets, 39,40 metal organic frameworks, 41 carbon dots, 42 and silica nanoparticles. 32 However, no such study has been reported using 2D MoS 2 nanosheets as supporting materials in spite of the outstanding catalytic performances exhibited by them. 19 In this work, we have used triblock copolymer P123-stabilized MoS 2 nanosheets as supporting materials for interfacing Cyt c and making a new nanobiocatalytic system with superior peroxidase-like catalytic activity. The MoS 2 nanosheets are of particular importance in this regard because: (1) they exhibit intrinsic peroxidase-like catalytic activity (therefore, they are often referred to as nanozymes) and (2) they can effectively interact with Cyt c, causing a conformational change to improve not only their own intrinsic catalytic activity but also the catalytic activity of Cyt c. 25 Therefore, the MoS 2 -nanozyme-activated synergistic amplification of the catalytic activity of our developed Cyt c−MoS 2 bionanohybrid catalyst is the major focus of the present work. Besides, we have also emphasized the understanding of the structural and conformational changes of the immobilized Cyt c on MoS 2 responsible for enhancing its catalytic efficiency. The peroxidase-like catalytic activity of the nanobiohybrid has been explored by probing the oxidation of a 2,2′-azino-bis-3-ethylbenzthiazoline-6-sulfonic acid (ABTS) substrate in the presence of another substrate H 2 O 2 . Cytochrome c from horse heart and sodium phosphate monobasic (anhydrous) and sodium phosphate dibasic (anhydrous) used to prepare phosphate buffer (PB) solution were purchased from Sisco Research Laboratories (SRL), India. All the reagents were used as received without further purification.
2.2. Preparation of MoS 2 Nanosheets. MoS 2 nanosheets were prepared by an ultrasonication-assisted centrifugation method. 10,43,44 In a typical experiment, 11 mg/mL of MoS 2 solution was prepared in 1% (w/v) aqueous pluronic P123 polymer solution, and the solution was sonicated for 5 h in a 100 W bath sonicator. Then the dispersed solution was subjected to centrifugation at 7000 rpm (in RM-12 Micro Centrifuge) to remove the bigger particles, and the supernatant was taken out as MoS 2 nanosheet dispersion. Nanosheet dispersions were found to be stable over several weeks.
2.3. Preparation of Cyt c−MoS 2 Nanobiohybrids. The Cyt c−MoS 2 nanobiohybrid was prepared through the spontaneous adsorption of Cyt c on P123 polymer functionalized MoS 2 nanosheets. First, we prepared stock solutions of MoS 2 (21 μg/mL) and Cyt c (100 μM) in aqueous 10 mM, pH 7.1 phosphate buffer. Appropriate amounts of the MoS 2 and Cyt c from their respective stock solutions were mixed in phosphate buffer to obtain a series of Cyt c−MoS 2 nanobiohybrid-containing solutions with increasing concentration (from 0.5 μg/mL to 3 μg/mL) of MoS 2 and a fixed 0.5 μM concentration of Cyt c. These solutions were used to study the MoS 2 concentration-dependent catalytic activity of the nanobiohybrids. The solutions were stirred for 5 min at room temperature before performing catalytic studies. The nanobiohybrids with 3 μg/mL of MoS 2 and 0.5 μM Cyt c were used for kinetic analysis by studying catalytic activities under varying substrate (ABTS/H 2 O 2 ) concentrations.
2.4. UV−vis Absorption, FTIR, and TEM Characterizations. UV−vis absorption studies of the MoS 2 nanosheets, Cyt c, and Cyt c−MoS 2 nanobiohybrids were performed using a spectrophotometer (model: LABINDIA-UV 3092). 44 The formation of the Cyt c−MoS 2 nanobiohybrid was confirmed by the observed shift of the Soret band position of Cyt c from 409 nm in the free native state to 400 nm in the bound state of the nanobiohybrids. The amount of Cyt c adsorbed on MoS 2 nanosheets was roughly estimated by spectrophotometric measurements of an aqueous buffer solution of Cyt c (10 μM) before and after addition of MoS 2 (10 μg/mL) into the solution. The decrease in absorbance of the free Cyt c at 409 nm (ε = 106 000 M −1 cm −1 ) due to the adsorption has been used to roughly estimate the concentration of the adsorbed Cyt c.
For FTIR studies of the MoS 2 nanosheets and the Cyt c− MoS 2 nanobiohybrids, the suspensions were centrifuged at higher rpms (around 12 000 rpm) multiple times and collected the solid particles. The solid particles were washed three to four times with distilled water to remove weakly adsorbed polymer molecules and dried at 56°C. The samples were analyzed with a Thermo Scientific-Nicolet iS5 FTIR spectrometer, in the frequency range of 500−4000 cm −1 . TEM measurement of the MoS 2 nanosheets was carried out using a JEM−2100 HRTEM (Make−JEOL, Japan) instrument. 25 2.5. Peroxidase Activity and Michaelis−Menten Kinetic Analysis. The peroxidase activity of immobilized Cyt c protein on MoS 2 was evaluated by measuring the initial rates of ABTS oxidation in the presence of H 2 O 2 . The formation of the oxidation product, the ABTS radical cation (ε 418 = 3.6 × 10 4 M −1 cm −1 ), was recorded by monitoring the time-dependent absorption increase at 418 nm. For the catalytic activity studies, a total 100 μL volume of the Cyt c−MoS 2 nanobiohybrid solution was taken in a cuvette (1 cm path length) and mixed with an appropriate concentration of ABTS (from a stock solution prepared in 10 mM phosphate buffer at pH 7.1). The absorption kinetics (at 418 nm) were started by the addition of H 2 O 2 . ABTS, H 2 O 2 , and nanobiohybrid samples were freshly prepared each time.
Peroxidase enzymatic kinetics of the Cyt c−MoS 2 nanobiohybrid (3 μg/mL of MoS 2 + 0.5 μM Cyt c) and MoS 2 (3 μg/mL) only systems as catalysts were analyzed using the Michaelis−Menten equation (eq 1), and the associated Lineweaver−Burk equation (eq 2) was used to obtain the kinetic parameters. In the Michaelis−Menten approach, the initial reaction rates (v 0 ) are measured at different initial substrate concentrations (S 0 ), and the kinetic parameters (V max , k cat , and K m ) are obtained from the linear fitting analysis of the Lineweaver−Burk plot (eq 2). In this work, the peroxidase-like catalytic cycle involves two substrates (H 2 O 2 and ABTS). To obtain the Michaelis−Menten kinetic parameters with respect to both the substrates, the Lineweaver−Burk plots have been constructed from a series of experiments in which the concentration of one of the substrate is held constant while varying the other one. The kinetic parameters obtained from this treatment are only apparent constants.
Here "v" is the initial reaction rate; "[S]" is the substrate concentration; "[E 0 ]" is the total enzyme concentration; k cat is the turnover rate constant; and K m is the Michaelis−Menten constant. 2.6. Molecular Docking Analysis. Docking analysis was carried out to observe any probable molecular interactions between the protein Cyt c and the PEO units of the triblock copolymer that are attached to the MoS 2 nanosheet surface. A ligand, 2-[2-(2-hydroxyethoxy)propoxy]ethanol, was docked on a horse heart Cyt c molecule using "Autodock Vina" software. Grid box dimensions were set to be 40 Å for X, Y, and Z conformations. To analyze the nature of substrate− protein binding interactions, the Cyt c molecule was also docked with ABTS and H 2 O 2 by the above procedure, in which the ligand was chosen as ABTS or H 2 O 2 .

RESULTS AND DISCUSSION
3.1. Spectroscopic and Microscopic Characterizations of MoS 2 Nanosheets. Figure 1a shows the absorption spectrum of MoS 2 nanosheet dispersion in aqueous P123 solution. The spectral characteristics share common features of the trigonal prismatic-coordinated 2H phase of MoS 2 . 45 The two characteristic absorption bands in the 600−700 nm region of the spectrum correspond to the excitonic transition of MoS 2 from the valence bands to the minima of the conductance band (at the K point of the Brillouin zone). The splitting of the valence band by spin−orbit and interlayer coupling interactions accounts for the two excitonic bands. 9,46 There are two additional higher energy absorption bands in the 350−450 nm region of the spectra corresponding to the transition of electrons to the higher density states of the Brillouin zone. 47 The concentration of the as-prepared MoS 2 nanosheet dispersion was calculated using the absorbance value at 345 nm, for which the extinction coefficient was previously reported as 6820 L g −1 cm −1 . 44 The concentration of the prepared nanosheet solution was found to be 21 μg/mL.
The FTIR spectrum of the P123 triblock copolymer coated MoS 2 nanosheets is given in Figure 1b. The corresponding spectra of the bulk MoS 2 material and the P123 polymer are given in Figure S1 of the Supporting Information. The FTIR results confirm that the surface of the MoS 2 nanosheets is functionalized with the P123 polymers. The presence of CH 3 groups of the central hydrophobic PPO blocks of the polymer on the MoS 2 nanosheets is confirmed by the two bands at ∼2965 and ∼1374 cm −1 . The 2965 cm −1 band can be assigned to the antisymmetric C−H stretching vibration of the methyl groups and the 1374 cm −1 band to the symmetric deformation band of the methyl groups. The FTIR peak at 2869 cm −1 corresponds to the antisymmetric methylene (CH 2 ) stretching modes. The 1093 cm −1 band is due to the C−O−C stretching vibration of the P123 polymer. These characteristic FTIR bands of the P123 polymer on the MoS 2 nanosheets are consistent with the FTIR spectrum of the pure P123 polymer ( Figure S1). 48 The other bands peaking at 1627 and 1260 cm −1 correlate well with the FTIR absorption bands of MoS 2 . 49 The TEM images of the P123 polymer stabilized MoS 2 nanosheets are given in Figure 1c,d. These images confirm the two-dimensional nanosheet structure of the synthesized MoS 2 . Moreover, the average dimension of the exfoliated individual nanosheets is found in the range of 90−100 nm.
3.2. Length and Thickness of the MoS 2 Nanosheets. The mean length and thickness of the MoS 2 nanosheets can be calculated using previously reported empirical relations based on the information at the characteristic A (at 660 nm) and B (at 610 nm) excitonic bands of the prepared MoS 2 nanosheets. The length of the MoS 2 nanosheet is related to the ratio of the extinction coefficient at the B-excitonic peak (E B ) to that at 345 nm (E 345 ) by the following relation: 44 The thickness of the nanosheets (referred to as number of MoS 2 layers in each nanosheet, N MoS 2 ) can be obtained from the peak position of the A-exciton band using the following relation: 44  Using the above relations, the calculated length and thickness of the MoS 2 nanosheets are found to be ∼90 nm and ∼3.4 layers/nanosheet, respectively. The calculated length of the MoS 2 nanosheets is found to be well correlated with the average dimension obtained from TEM results.
3.3. Characterization of the Cyt c−MoS 2 Nanobiohybrid System. The P123 stabilized MoS 2 nanosheets were used for the formation of a Cyt c−MoS 2 hybrid nanobiocatalytic system through the adsorption of Cyt c on the MoS 2 nanosheets. The formation of an interactive bionanointerface can be understood from UV−visible absorption spectral changes of Cyt c before and after adsorption on MoS 2 . Cyt c in its native oxidized state shows a highly intense Soret band at 409 nm and two other relatively low intense peaks around 522 and 360 nm named as Q and δ band, respectively (Figure 1a). The two visible region bands (Q and Soret bands) originate from the π to π* transitions of the porphyrin ring. 50 The Soret band is highly sensitive to the heme microenvironment of Cyt c. Any perturbations in and around heme will be reflected by the change in the peak position and/or intensity of the Soret band. 42 After being stirred with MoS 2 nanosheets, the Cyt c native Soret band position at 409 nm has been found to be blue-shifted to 400 nm. This clearly indicates possible interactions between Cyt c and the MoS 2 nanosheet template that might lead to some perturbations on the heme center suitable for peroxidase activity enhancement. Based on the decreased absorbance of the free native Cyt c at 409 nm upon adsorption on MoS 2 , the amount of adsorbed Cyt c on the MoS 2 nanosheets was estimated as 1.12 μM in 10 μg/mL of MoS 2 solution.
The influence of MoS 2 nanosheets on Cyt c is further supported by the FTIR analysis. The FTIR spectra of native Cyt c, the Cyt c−MoS 2 nanobiohybrid, and free MoS 2 nanosheets are given in Figure 2. The major characteristic amide I peak of the protein that arises from the carbonyl functionality of the peptide linkage has been shifted from 1654 cm −1 in the native state to 1650 cm −1 in the nanobiohybrid state. A similar shift (from 1545 cm −1 in the native state to 1541 cm −1 in the hybrid state) is also observed for the amide II region of the protein in the FTIR spectra (Figure 2b). Based on the correlation between the amide I band positions and the secondary structure of the proteins, the 1654 cm −1 band can be attributed to the α-helices, and the bands in the lower-and higher-frequency regions at 1629 and 1675 cm −1 correspond to the vibrations in β-sheet structure. Any major changes (position and intensity) of the amide I and II absorption bands are considered to be associated with the protein's secondary structural variations. 50 Ye et al. previously reported a similar FTIR spectral shift (from 1653 to 1649 cm −1 ) with a concomitant decrease in intensity of the amide I band of Cyt c upon increasing temperature. 51 This was assigned to the partial unfolding of the protein segment containing Met-80 which led to the disruption of the S−Fe bond at the heme coordination site. A similar structural perturbation can be expected for the Cyt c upon binding with MoS 2 . Such minor structural changes at the heme center are suitable for the activation of the peroxidase-like behavior of Cyt c. However, a major structural deviation or a complete unfolding would conversely affect protein's catalytic activity.
3 A binding energy of −3.7 kcal mol −1 was obtained for the best docking conformation of the protein with the ligand. The hydroxy-ethoxy moiety mainly exhibits polar hydrogen bonding interactions with the neighboring amino acids of the protein, such as arginine 38, glycine 23, histidine 33, glycine 34, and asparagine 31, either directly or through water molecules ( Figure S2). Some nonpolar interactions can be observed from a central propoxy moiety which is relatively hydrophobic in nature. Parray et al. 45 have recently indicated that the interaction of Cyt c with polyethylene glycol (with an interaction energy of −3.9 kcal mol −1 ) does not significantly perturb the Met 80-heme structure of Cyt c, meaning that the protein binds to PEG without major structural deviations. In the P123-supported MoS 2 system, the PEO (PEG) units provide a soft template for protein binding interactions and help to prevent major structural changes of Cyt c.  system. To understand the role of interactions between Cyt c and MoS 2 in modulating the catalytic activity of the hybrid system, we have also performed the catalytic oxidation of ABTS using free Cyt c and the MoS 2 nanosheets separately. The quantitative analysis of the catalysis was obtained from the time-dependent absorbance changes of the solutions at 418 nm, which is the characteristic absorption wavelength maximum of the ABTS radical cation formed during the reaction. The increase in absorbance (at 418 nm) with increasing time corresponds to an increase in concentration of the ABTS radical and thus provides kinetic information about the catalysis. Figure 3a shows the absorption kinetic curves recorded immediately after addition of 5 mM H 2 O 2 to a series of reaction solutions containing fixed concentrations of ABTS (0.5 mM) and Cyt c (0.5 μM) with an increasing concentration (0−3.0 μg/mL) of MoS 2 nanosheets in 10 mM phosphate buffer of pH 7.1. Before H 2 O 2 addition, the solutions were stirred and equilibrated for 5 min to ensure sufficient adsorption of Cyt c on MoS 2 nanosheets for effective catalysis reaction. The background absorptions of the reaction solutions before H 2 O 2 addition were subtracted to get the actual concentration of the ABTS radical cation formed at any given time of the reaction by converting the absorbance values into concentration using an extinction coefficient of 3.6 × 10 4 M −1 cm −1 of the radical cation at 418 nm. 39,52 In the absence of MoS 2 , free Cyt c resulted in only a slight increase in absorbance at 418 nm (over 300 s reaction time), suggesting weak peroxidase activity of free Cyt c in solution (Figure 3a). This is consistent with previous reports. 41 The peroxidase activity of the free Cyt c remains unchanged in the presence of 1% (w/v) P123 polymer, which has been used to stabilize the MoS 2 nanosheets ( Figure S3a). However, the presence of P123 polymer coated MoS 2 nanosheets as a supporting system significantly enhances the extent of absorbance increase (over the same reaction time) with a faster kinetics of ABTS radical cation formation. As the concentration of MoS 2 nanosheets increases from 0 to 3 μg/ mL, the absorbance at 418 nm at 300 s reaction time is increased linearly without leveling off (Figure 3b).
It is noteworthy to mention that, like graphene oxide, 53 MoS 2 nanosheets are also intrinsically active toward peroxidase catalysis, and the activity is highly dependent on the nature of surface modifications, as recently reported by Yu et al. 25 Therefore, we have studied the catalytic activity of our Weak peroxidase activity of native Cyt c can be attributed to the lower accessibility of the substrate to the six-coordinated structure with a low spin heme center protected by its native protein environment. 40,54 This is in contrast to that of a true peroxidase where a five-coordinated heme center with an almost vacant or loosely bound sixth coordination site allows easy access to the substrate to initiate peroxidase activity. 37 The enhanced peroxidase-like catalytic activity of Cyt c on MoS 2 can be due to the structure−function switching of Cyt c from its typical redox protein state into a well-performing peroxidase mimic. The interaction of Cyt c with the MoS 2 nanosheets probably led to partial unfolding of Cyt c with the slight perturbation of the heme structure, making the active site accessible to the substrates. The structural perturbation of the heme environment of Cyt c upon interactions with the MoS 2 nanosheets has already been confirmed from the UV− visible and FTIR analysis.
The MoS 2 nanosheets are known to have surface negative charge. Quinn et al. 43 previously reported a low negative surface charge (an approximate zeta potential of −13 mV) of the pluronic triblock copolymer supported MoS 2 nanosheets at pH 6.5. Based on this, the initial adsorption of the positively charged protein Cyt c on MoS 2 can be influenced by electrostatic attraction forces. However, as the MoS 2 nanosheet surface is covered with nonionic polymer P123, the hydrogen bonding and hydrophobic interactions between the polymer units (PEO and PPO moieties) and Cyt c will also play The influence of electrostatic forces on the peroxidase catalytic activity of the nanobiohybrid system was studied with the addition of 1 M NaCl into the reaction mixture ( Figure  S4a). The catalytic activity of the nanobiohybrid catalyst is found to be only slightly decreased in the presence of 1 M NaCl. For a better understanding, we have plotted the catalytic rate vs time curves in the absence and presence of 1 M NaCl as given in Figure S4b. From this figure, we can see that the decrease in catalytic activity is more pronounced at the initial reaction time (0−50 s), suggesting the influence of electrostatic forces at the initial stage of the reaction. At longer reaction time (50−300 s), the reactions in the absence and presence of NaCl converges to a state where the catalytic reaction progresses at a similar reaction velocity of 0.05 μM s −1 . Therefore, it can be inferred that increasing ionic strength reduces the initial activity through electrostatic forces, thereby leading to slightly lower concentration of the ABTS •+ formed at any equal time points. A strong influence of electrostatic forces on the catalytic activity was earlier reported for Cyt c on graphene oxide because of the presence of various ionizable polar groups on graphene oxide. 39,40 The effect of pH on the catalytic activity of the Cyt c−MoS 2 nanobiocatalyst was studied by preparing the reaction mixtures in phosphate buffers of pH 3.7, 7.1, and 10.3 ( Figure S5a). The catalytic activity of the Cyt c−MoS 2 nanobiohybrid significantly increases with decreasing pH of the medium. A similar trend is also observed for the control experiments using Cyt c (without MoS 2 ) and MoS 2 (without Cyt c) as catalysts ( Figure  S5b,c). Acidic pH enhances the peroxidase activity, whereas the basic pH significantly reduces the activity. However, in any particular pH condition, the catalytic activity of the Cyt c− MoS 2 nanobiohybrid is significantly higher than the activity of the individual components, MoS 2 and Cyt c ( Figure S5). The acidic pH condition facilitates the approach of the negatively charged substrate ABTS to the MoS 2 nanosheets and thereby improves the catalytic activity. Moreover, in the case of the nanobiohybrid, the acidic pH conditions probably provide more favorable conditions for the adsorption of Cyt c on the MoS 2 surface. 39 Both MoS 2 and Cyt c separately exhibit negligible catalytic properties in basic pH, while a weak activity is observed for their nanobiohybrid. The observed pH dependence is consistent with the previous reports on the peroxidase-like activity using a wide variety of catalytic systems. Gao et al. 55 earlier reported an optimal pH of 3.5 for the intrinsic peroxidase-like activity of Fe 3 O 4 nanoparticles. The activity of a peroxidase enzyme HRP was also shown to be optimum in similar acidic regions.
3.6. Time-Dependent Study of Catalytic Activity. Time-dependent variations in the catalytic activity of Cyt c− MoS 2 nanobiohybrids were studied by monitoring the H 2 O 2mediated ABTS oxidation kinetics at different incubation times of Cyt c with MoS 2 . For this, a solution containing the nanobiohybrids was prepared by mixing 0.5 μM Cyt c and 3 μg/mL of MoS 2 in aqueous buffer solution and its catalytic activity was assessed at different incubation times up to 48 h after mixing. With increasing incubation time, the catalytic activity of the nanobiohybrid was found to be decreased (Figure 4a). This is evidenced by the slower kinetics of ABTS oxidation with a lower extent of absorbance increase observed at a longer incubation period compared to that observed at a shorter incubation period. The reduced catalytic activity of the Cyt c−MoS 2 hybrid at longer incubation time is also supported by the time-dependent decrease in intensity of the Soret band of Cyt c upon adsorption on MoS 2 (Figure 4b). Immediately after mixing Cyt c with MoS 2 (within 10−15 min), the generation of the Cyt c−MoS 2 bionanointerface has caused a blue shift of the Soret band from 409 nm (characteristic of the native Cyt c) to 400 nm. As a result, the Cyt c gets activated for effective peroxidase like behavior. As the incubation time progresses, the intensity of the resultant 400 nm absorption band is gradually reduced, consistent with the observed loss of peroxidase activity (Figure 4). At 24 h of incubation, the absorbance of Cyt c is significantly reduced, and consequently the catalytic activity is dramatically decreased. This can be due to the degradation of the protein after a long incubation period (24 and 48 h).
3.7. Michaelis−Menten Kinetic Analysis. The catalytic activity of the Cyt c−MoS 2 bionanohybrid catalyst presented in this work can be viewed as a bisubstrate-based peroxidase-like catalysis reaction. The ABTS substrate is oxidized in the presence of another substrate H 2 O 2 , producing the ABTS radical cation (ABTS •+ ) as the product. Previously, multiple irreversible reaction steps were used to describe the peroxidase catalysis as shown in Scheme 2. 56 The first step of the peroxidase cycle involves a rapid two-electron oxidation of the catalyst by H 2 O 2 , producing an intermediate Compound I.
Compound I is converted back to the catalyst by two successive electron transfer reactions from the ABTS substrate (Scheme 2). The first step is reported to be highly rapid, and therefore, the rate of product formation is largely dependent on the reducing substrate ABTS. 56 In the case of horseradish peroxidase isoenzyme C, the rate constants follow the order k a > k b ≫ k c . 57 In the above model, the kinetic steps are considered as irreversible, assuming a linear kinetics of product formation. However, a large number of recent reports have suggested the reversible nature of the binding of H 2 O 2 to the enzyme before forming the intermediate compound I, justifying the applicability of the Michaelis−Menten kinetic model with evidence of saturated kinetics in peroxidase-like catalytic activities. 25,32,38,39,41 Here we have analyzed the kinetic data for the peroxidase activity of the Cyt c−MoS 2 nanobiohybrid catalyst with ABTS−H 2 O 2 as a dual substrate system using the Michaelis−Menten theory by applying eqs 1 and 2. To obtain the kinetic parameters using this model, the steady-state reaction kinetics were monitored by varying substrate concentration. The ABTS concentration variation (from 0.2 to 1 mM) kinetics assay was performed by keeping the H 2 O 2 fixed at an excess concentration of 5 mM (Figure 5a). Similarly, for the kinetics assay measurements with varying H 2 O 2 concentration (from 2 to 10 mM), the ABTS concentration was kept fixed at 0.5 mM ( Figure S6a). The absorbance kinetics were converted into the time-dependent concentration changes of the ABTS radical cation by using the molar extinction coefficient of the ABTS radical cation (ε 418 = 3.6 × 10 4 M −1 cm −1 ). The apparent steady-state reaction rates at the initial stage of the reaction at different substrate concentrations were obtained from the initial slope of the concentration kinetic curves. The initial reaction rates (v) vs substrate concentration plots were found to be hyperbolic (Figures 5b and S6b).
The Lineweaver−Burk plots ( Figure 6) exhibit linear characteristics, suggesting that the catalytic behavior of the Cyt c−MoS 2 nanobiohybrid follows the Michaelis−Menten enzymatic kinetics for both the ABTS and H 2 O 2 as substrates. The fitting analysis of the Lineweaver−Burk plots is provided by the Michaelis−Menten kinetic parameters, as given in Table   1. The Michaelis−Menten constant (K m ) is inversely related to the catalyst−substrate binding affinity. A lower K m value is desirable for a newly designed catalyst to obtain higher catalytic efficiency (k cat /K m ). 39 The K m values of the Cyt c− MoS 2 nanobiohybrid catalyst are found to be 1.20 and 2.94 mM for the ABTS and H 2 O 2 substrates, respectively. Similar low K m values were earlier reported for the peroxidase activity of Cyt c using graphene oxide, silica nanoparticles, and polymer scaffold as supporting systems. 32,38,39 The K m value of the Cyt c−MoS 2 nanobiohybrid is significantly lower than that of the free Cyt c (123 mM). 41 This suggests that Cyt c has a higher substrate binding affinity when adsorbed on the MoS 2 nanosheets.
Consistent with the literature reports, a lower K m value is observed for the nanobiocatalyst against the ABTS substrate compared to the H 2 O 2 substrate, indicating more profound catalyst−ABTS binding affinity than catalyst−H 2 O 2 binding. 39 This is primarily due to the electrostatic interactions between the negatively charged ABTS substrate and the positively charged Cyt c that are adsorbed on the surface of the P123 coated MoS 2 nanosheets at a physiological pH. This concentration fixed at 5 mM ( Figure S8). On the other hand, the H 2 O 2 concentration variation kinetic assay was obtained in the range 0.02−2 mM, keeping the ABTS concentration fixed at 0.5 mM ( Figure S9). The MoS 2 nanosheets (3 μg/mL) without Cyt c exhibit Michaelis−Menten kinetic behavior for both the substrates. This is evidenced from the hyperbolic plots of the initial rate vs substrate concentration as given in Figures S8b and S9b. The kinetic parameters obtained from the linear Lineweaver−Burk plots ( Figure S10) are given in Table 1. The catalytic efficiency (k cat /K m ) values of the P123 stabilized MoS 2 nanosheets alone are found to be around 109 and 106 for the ABTS and H 2 O 2 substrates, respectively. The catalytic efficiency of the MoS 2 nanosheets alone is significantly weaker than the corresponding Cyt c−MoS 2 nanobiohybrid. Therefore, free MoS 2 nanosheets alone only weakly contribute to the enhanced peroxidase activity of the Cyt c−MoS 2 nanobiohybrid.
3.8. Reaction Progress Kinetic Analysis. The peroxidase-like catalytic cycle involves two substrates (H 2 O 2 and ABTS) with multiple reaction steps. The kinetic analysis of such multistep-and multisubstrate-based catalytic reactions is complicated. The Michaelis−Menten kinetic model has been extensively applied to describe peroxidase-like catalytic activity for a wide variety of catalysts. However, it is important to note that the kinetic parameters (V max and K m ) obtained from this analysis for varying initial concentrations of a particular substrate will be dependent on the concentration of the other substrate. Thus, the obtained Michaelis−Menten kinetic parameters are considered to be only apparent constants. This can be better understood if we consider a simple possible mechanism for a bisubstrate-based catalytic cycle, as given in Scheme 3.
The rate of the reaction as derived under pseudo-steadystate conditions is given by (eq 5): Under the conditions of varying concentrations of both the substrates during the reaction, the reaction−progress−kinetic (RPK) analysis 58 provides an important understanding about the reaction mechanism and the orders of the reaction. In this graphical method, one needs to plot reaction rate vs substrate concentration by combining the substrate concentration vs time and the reaction rate vs time plots. In our peroxidase-like catalysis experiment, we record the accumulation of the product (ABTS •+ ) concentration (in terms of its absorbance) with increasing time. The rate vs time data were obtained by differentiating the product concentration vs time data. On the other hand, the substrate concentration vs time data were created by subtracting the product concentration vs time data  from the initial substrate concentration used in the reaction. By combining the rate vs time data and substrate concentration vs time data, we obtained the rate vs substrate concentration plot ( Figure S11) for the catalytic system with 1 mM ABTS, 5 mM H 2 O 2 , and 0.5 μM Cyt c supported on 3 μg/mL of MoS 2 as a catalyst. It is important to note that this plot describes the rate of the catalytic reaction as the ABTS substrate is consumed from right to left because the substrate concentration decreases from the initial concentration as the product forms over the course of the reaction. The plot shows a curved feature, indicating a complex relationship between the rate and the substrate ABTS as described in the rate equation (eq 5).
We have applied variable-time-normalization analysis (VTNA) following a reported procedure to find the order of the reaction with respect to the hybrid catalyst. 59 In this analysis, the time scale of the two reactions run with different catalyst loadings is substituted by the normalized time scale, ∑[C] γ Δt (eq 7).
where [C] is the concentration of the catalyst, and the value of "γ" that produces the overlay of the curves is the order in catalyst. The normalization term is based on the fact that the concentration of the catalyst is constant during the entire reaction without any deactivation. We have used this "constant normalization" of the time scale method to overlay the curves of two different kinetic profiles recorded using two different concentrations of the catalyst (3 and 2 μg/mL of MoS 2 with a fixed 0.5 μM of Cyt c). The overlay analysis of the curves in this concentration range of the MoS 2 gave the order of the reaction with respect to the catalyst as 2 ( Figure S12).

CONCLUSION
In conclusion, a new nanobiocatalytic system has been prepared through the spontaneous adsorption of Cyt c on a triblock copolymer, P123, stabilized MoS 2 nanosheet. The catalytic activity of these nanobiohybrid systems has been successfully demonstrated by studying H 2 O 2 -mediated oxidation of the ABTS substrate. The enhanced catalytic performance of the Cyt c−MoS 2 nanobiohybrid catalyst compared to that of the free Cyt c and MoS 2 nanosheets can be explained based on the minor structural perturbation of the active site of the Cyt c upon adsorption on MoS 2 nanosheets. The triblock copolymer support on the MoS 2 nanosheets plays an important role in protecting the proteins from undergoing major structural changes. Moreover, the polymer support attracts more proteins to be adsorbed on the MoS 2 nanosheets and thereby increases the catalytic performance. From the study of Michaelis−Menten kinetics analysis, it is revealed that the adsorption of Cyt c on P123 stabilized MoS 2 nanosheets significantly increases the substrate binding affinity as well as the catalytic efficiency. Such a nanobiocatalytic system exhibiting high stability with enhanced catalytic activity may find their potential applications in biosensing, biofuel cells, and biomedical fields.